Polytetrafluoroethylene (PTFE) is a synthetic fluoropolymer of tetrafluoroethylene that has numerous applications. The best known brand name of PTFE-based formulas is Teflon by Chemours. Chemours is a 2015 spin-off of DuPont Co., which discovered the compound in 1938.
Syncolon, Fluon, Poly(tetrafluroethene), Poly(difluoromethylene), Poly(tetrafluoroethylene)
|Melting point||600 K|
|Thermal conductivity||0.25 W/(m·K)|
Except where otherwise noted, data are given for materials in their standard state (at 25 °C [77 °F], 100 kPa).
|what is ?)(|
PTFE is a fluorocarbon solid, as it is a high-molecular-weight compound consisting wholly of carbon and fluorine. PTFE is hydrophobic: neither water nor water-containing substances wet PTFE, as fluorocarbons demonstrate mitigated London dispersion forces due to the high electronegativity of fluorine. PTFE has one of the lowest coefficients of friction of any solid.
PTFE is used as a non-stick coating for pans and other cookware. It is nonreactive, partly because of the strength of carbon–fluorine bonds, and so it is often used in containers and pipework for reactive and corrosive chemicals. Where used as a lubricant, PTFE reduces friction, wear, and energy consumption of machinery. It is commonly used as a graft material in surgical interventions. Also, it is frequently employed as coating on catheters; this interferes with the ability of bacteria and other infectious agents to adhere to catheters and cause hospital-acquired infections.
|"From stove tops to outer space... Teflon touches every one of us some way almost every day.", Roy Plunkett, Science History Institute|
PTFE was accidentally discovered in 1938 by Roy Plunkett while he was working in New Jersey for DuPont. As Plunkett attempted to make a new chlorofluorocarbon refrigerant, the tetrafluoroethylene gas in its pressure bottle stopped flowing before the bottle's weight had dropped to the point signaling "empty." Since Plunkett was measuring the amount of gas used by weighing the bottle, he became curious as to the source of the weight, and finally resorted to sawing the bottle apart. He found the bottle's interior coated with a waxy white material that was oddly slippery. Analysis showed that it was polymerized perfluoroethylene, with the iron from the inside of the container having acted as a catalyst at high pressure. Kinetic Chemicals patented the new fluorinated plastic (analogous to the already known polyethylene) in 1941, and registered the Teflon trademark in 1945.
By 1948, DuPont, which founded Kinetic Chemicals in partnership with General Motors, was producing over two million pounds (900 tons) of Teflon brand PTFE per year in Parkersburg, West Virginia. An early use was in the Manhattan Project as a material to coat valves and seals in the pipes holding highly reactive uranium hexafluoride at the vast K-25 uranium enrichment plant in Oak Ridge, Tennessee.
In 1954, the wife of French engineer Marc Grégoire urged him to try the material he had been using on fishing tackle on her cooking pans. He subsequently created the first PTFE-coated, non-stick pans under the brandname Tefal (combining "Tef" from "Teflon" and "al" from aluminium). In the United States, Marion A. Trozzolo, who had been using the substance on scientific utensils, marketed the first US-made PTFE-coated pan, "The Happy Pan", in 1961.
However, Tefal was not the only company to utilize PTFE in nonstick cookware coatings. In subsequent years, many cookware manufacturers developed proprietary PTFE-based formulas, including Swiss Diamond International, which uses a diamond-reinforced PTFE formula; Scanpan, which uses a titanium-reinforced PTFE formula; and both All-Clad and Newell Rubbermaid's Calphalon, which use a non-reinforced PTFE-based nonstick. Other cookware companies, such as Meyer Corporation's Anolon, use Teflon nonstick coatings purchased from DuPont. Newer cookware brands, such as Made In, are also using a no-PFOA version of PTFE.
In the 1990s, it was found that PTFE could be radiation cross-linked above its melting point in an oxygen-free environment. Electron beam processing is one example of radiation processing. Cross-linked PTFE has improved high-temperature mechanical properties and radiation stability. This was significant because, for many years, irradiation at ambient conditions has been used to break down PTFE for recycling. This radiation-induced chain scission allows it to be more easily reground and reused.
- n F2C=CF2 → −(F2C−CF2)n−
Because tetrafluoroethylene can explosively decompose to tetrafluoromethane and carbon, special apparatus is required for the polymerization to prevent hot spots that might initiate this dangerous side reaction. The process is typically initiated with persulfate, which homolyzes to generate sulfate radicals:
- [O3SO−OSO3]2− ⇌ 2 SO4•−
Because PTFE is poorly soluble in almost all solvents, the polymerization is conducted as an emulsion in water. This process gives a suspension of polymer particles. Alternatively, the polymerization is conducted using a surfactant such as PFOS.
PTFE is a thermoplastic polymer, which is a white solid at room temperature, with a density of about 2200 kg/m3. According to Chemours, its melting point is 600 K (327 °C; 620 °F). It maintains high strength, toughness and self-lubrication at low temperatures down to 5 K (−268.15 °C; −450.67 °F), and good flexibility at temperatures above 194 K (−79 °C; −110 °F). PTFE gains its properties from the aggregate effect of carbon-fluorine bonds, as do all fluorocarbons. The only chemicals known to affect these carbon-fluorine bonds are highly reactive metals like the alkali metals, and at higher temperatures also such metals as aluminium and magnesium, and fluorinating agents such as xenon difluoride and cobalt(III) fluoride.
|Glass temperature||114.85 °C (238.73 °F; 388.00 K) |
|Melting point||326.85 °C (620.33 °F; 600.00 K)|
|Thermal expansion||112–125 · 10−6 K−1 |
|Thermal diffusivity||0.124 mm2/s |
|Young's modulus||0.5 GPa|
|Yield strength||23 MPa|
|Bulk resistivity||1016 Ω·m |
|Coefficient of friction||0.05–0.10|
|Dielectric constant||ε = 2.1, tan(δ) < 5(-4)|
|Dielectric constant (60 Hz)||ε = 2.1, tan(δ) < 2(-4)|
|Dielectric strength (1 MHz)||60 MV/m|
|Magnetic Susceptibility (SI, 22 °C)||−10.28×10−6 |
The coefficient of friction of plastics is usually measured against polished steel. PTFE's coefficient of friction is 0.05 to 0.10, which is the third-lowest of any known solid material (BAM being the first, with a coefficient of friction of 0.02; diamond-like carbon being second-lowest at 0.05). PTFE's resistance to van der Waals forces means that it is the only known surface to which a gecko cannot stick. In fact, PTFE can be used to prevent insects climbing up surfaces painted with the material. PTFE is so slippery that insects cannot get a grip and tend to fall off. For example, PTFE is used to prevent ants climbing out of formicaria.
Because of its chemical inertness, PTFE cannot be cross-linked like an elastomer. Therefore, it has no "memory" and is subject to creep. Because of its superior chemical and thermal properties, PTFE is often used as a gasket material within industries that require resistance to aggressive chemicals such as pharmaceuticals or chemical processing. However, because of the propensity to creep, the long-term performance of such seals is worse than for elastomers which exhibit zero, or near-zero, levels of creep. In critical applications, Belleville washers are often used to apply continuous force to PTFE gaskets, ensuring a minimal loss of performance over the lifetime of the gasket.
Processing PTFE can be difficult and expensive, because the high melting temperature, 327 °C (621 °F), is above the initial decomposition temperature, 200 °C (392 °F). Even when melted, PTFE does not flow, but instead behaves as a gel due to the absence of crystalline phase and high melt viscosity.
Some PTFE parts are made by cold-moulding, a form of compression molding. Here, fine powdered PTFE is forced into a mould under high pressure (10 ~ 100 MPa). After a settling period, lasting from minutes to days, the mould is heated at 360 to 380 degrees Celsius (680 to 716 degrees Fahrenheit), allowing the fine particles to fuse into a single mass.
Applications and usesEdit
This section needs additional citations for verification. (May 2017) (Learn how and when to remove this template message)
The major application of PTFE, consuming about 50% of production, is for wiring in aerospace and computer applications (e.g. hookup wire, coaxial cables). This application exploits the fact that PTFE has excellent dielectric properties, especially at high radio frequencies, making it suitable for use as an excellent insulator in connector assemblies and cables, and in printed circuit boards used at microwave frequencies. Combined with its high melting temperature, this makes it the material of choice as a high-performance substitute for the weaker and lower-melting-point polyethylene commonly used in low-cost applications.
In industrial applications, owing to its low friction, PTFE is used for plain bearings, gears, slide plates, seals, gaskets, bushings, and more applications with sliding action of parts, where it outperforms acetal and nylon.
PTFE film is also widely used in the production of carbon fiber composites as well as fiberglass composites, notably in the aerospace industry. PTFE film is used as a barrier between the carbon or fiberglass part being built, and breather and bagging materials used to incapsulate the bondment when debulking (vacuum removal of air from between layers of laid-up plies of material) and when curing the composite, usually in an autoclave. The PTFE, used here as a film, prevents the non-production materials from sticking to the part being built, which is sticky due to the carbon-graphite or fiberglass plies being pre-pregnated with bismaleimide resin. Non-production materials such as Teflon, Airweave Breather and the bag itself would be considered F.O.D. (foreign object debris/damage) if left in layup.
Because of its extreme non-reactivity and high temperature rating, PTFE is often used as the liner in hose assemblies, expansion joints, and in industrial pipe lines, particularly in applications using acids, alkalis, or other chemicals. Its frictionless qualities allow improved flow of highly viscous liquids, and for uses in applications such as brake hoses.
Gore-Tex is a brand of expanded PTFE (ePTFE), a material incorporating a fluoropolymer membrane with micropores. The roof of the Hubert H. Humphrey Metrodome in Minneapolis, US, was one of the largest applications of PTFE coatings. 20 acres (81,000 m2) of the material was used in the creation of the white double-layered PTFE-coated fiberglass dome.
PTFE is often found in musical instrument lubrication product; most commonly, valve oil.
PTFE is used in some aerosol lubricant sprays, including in micronized and polarized form. It is notable for its extremely low coefficient of friction, its hydrophobia (which serves to inhibit rust), and for the dry film it forms after application, which allows it to resist collecting particles that might otherwise form an abrasive paste. 
The sole plates of some clothes irons are coated with PTFE (Teflon).
Other niche applications include:
- It is often found in ski bindings as a non-mechanical AFD (Anti-Friction Device)
- It can be stretched to contain small pores of varying sizes and is then placed between fabric layers to make a waterproof, breathable fabric in outdoor apparel.
- It is used widely as a fabric protector to repel stains on formal school-wear, like uniform blazers.
- It is used as a film interface patch for sports and medical applications, featuring a pressure-sensitive adhesive backing, which is installed in strategic high friction areas of footwear, insoles, ankle-foot orthosis, and other medical devices to prevent and relieve friction-induced blisters, calluses and foot ulceration.
- Expanded PTFE membranes have been used in trials to assist trabeculectomy surgery to treat glaucoma.
- Powdered PTFE is used in pyrotechnic compositions as an oxidizer with powdered metals such as aluminium and magnesium. Upon ignition, these mixtures form carbonaceous soot and the corresponding metal fluoride, and release large amounts of heat. They are used in infrared decoy flares and as igniters for solid-fuel rocket propellants. Aluminium and PTFE is also used in some thermobaric fuel compositions.
- Powdered PTFE is used in a suspension with a low-viscosity, azeotropic mixture of siloxane ethers to create a lubricant for use in twisty puzzles.
- In optical radiometry, sheets of PTFE are used as measuring heads in spectroradiometers and broadband radiometers (e.g., illuminance meters and UV radiometers) due to PTFE's capability to diffuse a transmitting light nearly perfectly. Moreover, optical properties of PTFE stay constant over a wide range of wavelengths, from UV down to near infrared. In this region, the ratio of its regular transmittance to diffuse transmittance is negligibly small, so light transmitted through a diffuser (PTFE sheet) radiates like Lambert's cosine law. Thus PTFE enables cosinusoidal angular response for a detector measuring the power of optical radiation at a surface, e.g. in solar irradiance measurements.
- Certain types of bullets are coated with PTFE to reduce wear on the rifling of firearms that uncoated projectiles would cause. PTFE itself does not give a projectile an armor-piercing property.
- Its high corrosion resistance makes PTFE useful in laboratory environments, where it is used for lining containers, as a coating for magnetic stirrers, and as tubing for highly corrosive chemicals such as hydrofluoric acid, which will dissolve glass containers. It is used in containers for storing fluoroantimonic acid, a superacid.
- PTFE tubes are used in gas-gas heat exchangers in gas cleaning of waste incinerators. Unit power capacity is typically several megawatts.
- PTFE is widely used as a thread seal tape in plumbing applications, largely replacing paste thread dope.
- PTFE membrane filters are among the most efficient industrial air filters. PTFE-coated filters are often used in dust collection systems to collect particulate matter from air streams in applications involving high temperatures and high particulate loads such as coal-fired power plants, cement production and steel foundries.
- PTFE grafts can be used to bypass stenotic arteries in peripheral vascular disease if a suitable autologous vein graft is not available.
- Many bicycle lubricants and greases contain PTFE and are used on chains and other moving parts subjected to frictional forces (such as hub bearings).
- PTFE can also be used for dental fillings, to isolate the contacts of the anterior tooth so the filling materials will not stick to the adjacent tooth.
- PTFE sheets are used in the production of butane hash oil due to its non-stick properties and resistance to non-polar solvents.
- PTFE, associated with a slightly textured laminate, makes the plain bearing system of a Dobsonian telescope.
- PTFE is widely used as a non-stick coating for food processing equipment; dough hoppers, mixing bowls, conveyor systems, rollers, and chutes. PTFE can also be reinforced where abrasion is present - for equipment processing seeded or grainy dough for example
- Has been experimented with for electroless nickel plating
Pyrolysis of PTFE is detectable at 200 °C (392 °F), and it evolves several fluorocarbon gases and a sublimate. An animal study conducted in 1955 concluded that it is unlikely that these products would be generated in amounts significant to health at temperatures below 250 °C (482 °F).
While PTFE is stable and nontoxic at lower temperatures, it begins to deteriorate after the temperature of cookware reaches about 260 °C (500 °F), and decomposes above 350 °C (662 °F). The degradation by-products can be lethal to birds, and can cause flu-like symptoms in humans—see polymer fume fever. Meat is usually fried between 204 and 232 °C (399 and 450 °F), and most oils start to smoke before a temperature of 260 °C (500 °F) is reached, but there are at least two cooking oils (refined safflower oil at 265 °C (510 °F) and avocado oil at 271 °C (520 °F)) that have a higher smoke point.
Perfluorooctanoic acid (PFOA, or C8) has been used as a surfactant in the emulsion polymerization of PTFE, although several manufacturers have entirely discontinued its use. PFOA persists indefinitely in the environment. It is a toxicant and carcinogen in animals. PFOA has been detected in the blood of more than 98% of the general US population in the low and sub-parts per billion range, and levels are higher in chemical plant employees and surrounding subpopulations. The general population has been exposed to PFOA through massive dumping of C8 waste into the ocean and near the Ohio River Valley. PFOA has been detected in industrial waste, stain resistant carpets, carpet cleaning liquids, house dust, microwave popcorn bags, water, food and Teflon cookware.
As a result of a class-action lawsuit and community settlement with DuPont, three epidemiologists conducted studies on the population surrounding a chemical plant that was exposed to PFOA at levels greater than in the general population. The studies concluded that there was probably an association between PFOA exposure and six health outcomes: kidney cancer, testicular cancer, ulcerative colitis, thyroid disease, hypercholesterolemia (high cholesterol), and pregnancy-induced hypertension.
The Teflon trade name is also used for other polymers with similar compositions:
These retain the useful PTFE properties of low friction and nonreactivity, but are more easily formable. For example, FEP is softer than PTFE and melts at 533 K (260 °C; 500 °F); it is also highly transparent and resistant to sunlight.
- "poly(tetrafluoroethylene) (CHEBI:53251)". ebi.ac.uk. Retrieved 12 July 2012.
- "Teflon ™| Chemours Teflon™ Nonstick Coatings and Additives". www.chemours.com. Retrieved 2016-03-01.
- "DuPont - DuPont Completes Spin-off of The Chemours Company". investors.dupont.com. Retrieved 2016-03-01.
- US 2230654, Plunkett, Roy J, "Tetrafluoroethylene polymers", issued 4 February 1941
- "History Timeline 1930: The Fluorocarbon Boom". DuPont. Retrieved 10 June 2009.
- "Roy Plunkett: 1938". Retrieved 10 June 2009.
- American Heritage of Invention & Technology, Fall 2010, vol. 25, no. 3, p. 42
- Rhodes, Richard (1986). The Making of the Atomic Bomb. New York, New York: Simon and Schuster. p. 494. ISBN 0-671-65719-4. Retrieved 31 October 2010.
- "Teflon History ", home.nycap.rr.com, Retrieved 25 January 2009.
- Robbins, William (21 December 1986) "Teflon Maker: Out Of Frying Pan Into Fame ", New York Times, Retrieved 21 December 1986 (Subscription)
- Swiss Diamond Technology Swiss Diamond International
- About SCANPAN SCANPAN
- FAQ's "Is Nonstick Safe," All-Clad FAQ
- FAQ's "Does your cookware contain Teflon®?" Calphalon FAQ
- Knowledge Base Analon
- "Frequently Asked Questions". Made In Cookware. Retrieved 2018-08-15.
- Sun, J.Z.; et al. (1994). "Modification of polytetrafluoroethylene by radiation—1. Improvement in high temperature properties and radiation stability". Radiat. Phys. Chem. 44 (6): 655–679. Bibcode:1994RaPC...44..655S. doi:10.1016/0969-806X(94)90226-7.
- Electron Beam Processing of PTFE E-BEAM Services website. Accessed 21 May 2013
- Carlson, D. Peter and Schmiegel, Walter (2000) "Fluoropolymers, Organic" in Ullmann's Encyclopedia of Industrial Chemistry, Wiley-VCH, Weinheim. doi:10.1002/14356007.a11_393
- Fluoroplastic Comparison - Typical Properties Retrieved 16 January 2018.
- Teflon PTFE Properties Handbook Retrieved 11 October 2012.
- DuPont Teflon® Coatings. plastechcoatings.com
- Nicholson, John W. (2011). The Chemistry of Polymers (4, Revised ed.). Royal Society of Chemistry. p. 50. ISBN 9781849733915.
- "Reference Tables – Thermal Expansion Coefficients – Plastics". engineershandbook.com.
- Blumm, J.; Lindemann, A.; Meyer, M.; Strasser, C. (2011). "Characterization of PTFE Using Advanced Thermal Analysis Technique". International Journal of Thermophysics. 40 (3–4): 311. Bibcode:2010IJT....31.1919B. doi:10.1007/s10765-008-0512-z.
- "PTFE". Microwaves101.
- Wapler, M. C.; Leupold, J.; Dragonu, I.; von Elverfeldt, D.; Zaitsev, M.; Wallrabe, U. (2014). "Magnetic properties of materials for MR engineering, micro-MR and beyond". JMR. 242: 233–242. arXiv:1403.4760. Bibcode:2014JMagR.242..233W. doi:10.1016/j.jmr.2014.02.005.
- Coefficient of Friction (COF) Testing of Plastics MatWeb Material Property Data Retrieved 1 January 2007.
- "Research into Gecko Adhesion ", Berkeley, 2007-10-14, Retrieved 8 April 2010.
- Inc., Gasket Resources. "PTFE Sheet | Gasket Resources Inc". www.gasketresources.com. Retrieved 2017-08-16.
- Davet, George P. "Using Belleville Springs To Maintain Bolt Preload" (PDF). Solon Mfg. Co. Retrieved 18 May 2014.
- Zapp JA, Limperos G, Brinker KC (26 April 1955). "Toxicity of pyrolysis products of 'Teflon' tetrafluoroethylene resin". Proceedings of the American Industrial Hygiene Association Annual Meeting.
- "Free Flow Granular PTFE" (PDF). Inoflon Fluoropolymers. 2017-08-16.
- "COWIE TECHNOLOGY - PTFE: High Thermal Stability". www.cowie.com. Retrieved 2017-08-16.
- "Polyflon PTFE Molding Powder" (PDF). Daikin Chemical. 2017-08-16.
- "Unraveling Polymers: PTFE". Poly Fouoro Ltd. 26 April 2011. Retrieved 23 April 2017.
- Mishra, Munmaya; Yagci, Yusuf (208). Handbook of Vinyl Polymers: Radical Polymerization, Process, and Technology, Second Edition (2nd, illustrated, revised ed.). CRC Press. p. 574. ISBN 978-0-8247-2595-2. Extract of page 574
- "Teflon Machining & Fabrication | ESPE". www.espemfg.com. Retrieved 2018-08-28.
- Mishra & Yagci, p 573
- "What is MicPol?". Lubrication. Retrieved 2018-10-03.
- Fers à repasser semelle teflon - Fiche pratique - Le Parisien. Pratique.leparisien.fr. Retrieved on 2016-11-17.
- "A Motorcyclist's Guide To Gore-Tex". Infinity Motorcycles.
- "Advantages and Disadvantages of Teflon-coated Covert Cloth". The Cutter and Tailor.
- "Film Interface Patch". American Academy of Orthotists & Prosthetists.
- Wang X, Khan R, Coleman A (2015). "Device-modified trabeculectomy for glaucoma". Cochrane Database Syst Rev. 12: CD010472. doi:10.1002/14651858.CD010472.pub2. PMC 4715269. PMID 26625212.
- Koch, E.-C. (2002). "Metal-Fluorocarbon Pyrolants:III. Development and Application of Magnesium/Teflon/Viton". Propellants, Explosives, Pyrotechnics. 27 (5): 262–266. doi:10.1002/1521-4087(200211)27:5<262::AID-PREP262>3.0.CO;2-8.
- "Lubicle 1". TheCubicle.us. Retrieved 2017-05-20.
- "Interview with an inventor of the KTW bullet". NRAction newsletter. 4 (5). May 1990.
- Pomeroy, Ross (2013-08-24). "The World's Strongest Acids: Like Fire and Ice". Retrieved 2016-04-09.
- "Industrial Air Permits - New Clean Air Regulations And Baghouses". Baghouse.com.
- Brown, DDS, Dennis E. "Using Plumber's Teflon Tape to Enhance Bonding Procedures". Dentistry Today.
- Dunn, WJ; et al. "Polytetrafluoroethylene (PTFE) tape as a matrix in operative dentistry". Operative Dentistry. 29: 470–2. PMID 15279489.
- Rosenthal, Ed (21 October 2014). Beyond Buds (Revised ed.). Quick American Archives. ISBN 1936807238.
- "Fluoropolymer PTFE coating services from Surface Technology UK". Surface Technology. Retrieved 2018-02-26.
- "Polytetrafluouroethylene: PTFE Sheets & PTFE Coatings from Porex". www.porex.com. Retrieved 2016-01-21.
- "Key Safety Questions About Teflon Nonstick Coatings". DuPont. Retrieved 28 November 2014.
- "Key Safety Questions about the Safety of Nonstick Cookware". DuPont.
- RIch, Nathaniel. "The Lawyer Who Became Dupont's Worst Nightmare". The New York Times Magazine. Retrieved 7 January 2016.
- Blake, Mariah. "Welcome to Beautiful Parkersburg, West Virginia Home to one of the most brazen, deadly corporate gambits in U.S. history". Huffington Post. Retrieved 31 August 2015.
- Fellner, Carrie (16 June 2018). "Toxic Secrets: Professor 'bragged about burying bad science' on 3M chemicals". Sydney Morning Herald. Retrieved 25 June 2018.
- Nicole, W. (2013). "PFOA and Cancer in a Highly Exposed Community: New Findings from the C8 Science Panel". Environmental Health Perspectives. 121 (11–12): A340. doi:10.1289/ehp.121-A340. PMC 3855507. PMID 24284021.
- Trudel D, Horowitz L, Wormuth M, Scheringer M, Cousins IT, Hungerbühler K (April 2008). "Estimating consumer exposure to PFOS and PFOA". Risk Anal. 28 (2): 251–69. doi:10.1111/j.1539-6924.2008.01017.x. PMID 18419647.
- "Nonstick pans: Nonstick coating risks". Consumer Reports. Retrieved 4 July 2009.
- FEP Detailed Properties, Parker-TexLoc, 13 April 2006. Retrieved 10 September 2006.
- EPA: Compound in Teflon may cause cancer , Tom Costello, NBC News, 29 June 2005. (Flash video required)
- Plasma Processes and Adhesive Bonding of Polytetrafluoroethylene
- PTFE Tubing Properties